SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES


 Imogene Ward
 1 years ago
 Views:
Transcription
1 SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK 2 Loughborough University, Department of Aeronautical and Automotive Engineering, LE11 3TU, UK, SUMMARY The paper presents a new methodology for identifying subsurface damage in composite components using a combination of Pulse Phase Thermography (PPT) and Thermoelastic Stress Analysis (TSA). Keywords: Composite structures, Thermoelastic Stress Analysis (TSA), Pulsed Phase Thermography (PPT), Damage INTRODUCTION The location and identification of damage in composite materials is currently a topic of considerable interest, and many techniques are being applied and developed in both the research and industrial communities in order to advance knowledge in the area. Infrared thermography (IRT) systems are now available that can collect data a high rates and allow the heating effects due to damage to be observed in real time. Thermoelastic Stress Analysis (TSA) [1] is a noncontacting, fullfield measurement technique that uses IRT as its basis and has been shown to have great potential for use in damage assessment studies. In TSA, IRT is used to obtain the small temperature change that occurs as a result of a strain change in the structure. It is now possible to monitor the evolution of damage in real time using TSA. It is also possible to decouple the part of the thermoelastic response caused by heating at the damage site from the response produced by the strain change [2]. Therefore TSA can now be applied as a quantitative tool for damage assessment. The difficulty with TSA is that it is essentially a surface technique and in many cases damage evolves from subsurface defects and/or delaminations. Pulse Phase Thermography (PPT) is a relatively new approach that combines pulse and modulated thermography [3]. The main advantage of the PPT approach is that it has the potential to reveal subsurface damage. It is also portable, so that inspections of components that are inservice can take place. Furthermore it is relatively fast, so that inspections of large components can be carried out to pinpoint areas of damage for further analysis, using a technique such as TSA. The purpose of this paper is to define a methodology where PPT is used to detect, locate and identify the extent of subsurface delamination damage and then TSA is used to characterise the effect of the damage on the stress field in the component.
2 Thermoelastic Stress Analysis TSA is an experimental technique that is based on the well documented thermoelastic effect, e.g. [4, 5]. The technique uses a highly sensitive infrared (IR) detector to measure the small temperature changes (of the order of mk) within the field of view that can in turn be related to the change in the sum of the principal stresses x y, as follows: T T ( x y ) (1) C p where is the coefficient of linear thermal expansion, T is the absolute temperature, is the density and C p is the specific heat at constant pressure. The analogue output from the IR detector is digitally processed into the thermoelastic signal (S) and is related to the change in the sum of the principal stresses using a calibration constant (A) which can be experimentally determined [6], as follows [7]: AS (2) x y Equation (2) is applicable for an isotropic homogeneous material. Orthotropic materials have markedly different mechanical properties in the principal material directions and consequently the simple thermoelastic theory devised for an isotropic body is not valid for orthotropic composite materials [8]. The thermoelastic theory has been developed [8] into an equation for an orthotropic homogeneous material as follows: A* S (3) where 1 and 2 are the coefficients of linear thermal expansion in the principal material directions, Δ 1 and Δ 2 are the changes in the direct surface stresses in the principal material directions and A* is an orthotropic calibration constant. The technique has not been widely applied to the assessment of composite structures due to the difficulties presented by the material anisotropic behaviour. However, with recent developments in the instrumentation, that has allowed more detailed data to be gathered in virtually real time, the incentive to apply TSA to damage studies of composite components has been provided. Through calibration of the signal, the output can be related to the stresses in the structure and therefore life assessments may be possible. Equation (3) is developed [8] in terms of the principal surface stresses. To calibrate the thermoelastic theory it is therefore necessary to obtain values of the surface stress. In laminated composite materials this can be achieved by applying classical laminate theory (CLT) provided the elastic properties of the lamina, the thickness of the manufactured plies and the loads are known. This can provide a route to calibration [9] based on Equation (3) but is laden with possible sources of error due to estimates of material properties etc. A better approach is to formulate Equation (3) in terms of strain, which leads to:
3 1Q11 2Q12 1 1Q12 2Q22 2 A * S (4) where 1 and 2 are the coefficients of thermal expansion in the surface lamina relative fibre directions, Q 11, Q 12, and Q 22 are the laminate reduced stiffness terms [10], and 1 and 2 are the surface lamina strains in the relative fibre directions. This equation can also be rewritten in terms of the strains in the laminate principal material directions (L and T directions) using the strain transformation equations [10]. This formulation provides a direct approach to calibration, as the strain is constant through the thickness of a laminate and furthermore can be measured using extensometers or strain gauges. Pulse Phase Thermography PPT is a relatively new approach that combines the traditional IRT techniques of pulse (PT) and modulated thermography (MT) [11]. It is a passive technique and therefore can be applied to large areas of inservice composite structures. Furthermore, it is relatively fast, so that inspections of large components can be carried out to pinpoint areas of damage for further analysis. PPT is achieved by subjecting the structure under evaluation to a pulse of heat energy that propagates through the structure and subsequently analysing the thermal signature from the surface. A sequence of IR images is collected from the surface following the thermal pulse that captures the thermal decay T(t). Mathematically the thermal pulse can be decomposed into a multitude of individual sinusoidal components [11] with various amplitudes and frequencies. The frequency content of these sinusoidal components, that diffuse through the structure and appear on the surface, can be obtained from the thermal images recorded using Fourier transformation analysis. The extraction and comparison of various specified frequency ranges, using a discrete onedimensional Fourier transform at each pixel in the image, provides the basis for PPT. The frequency range analysed is dependent on the damage location and geometry within the specimen. The output is provided in terms of the amplitude and phase of the frequency wave at the surface. The output is referenced relative to each pixel, at time t, in the field of view and as such no reference input is required but any change in transmission evident at the surface can be evaluated. Phase lag or attenuation, of the wave in question, at a pixel relative to another pixel will be evident in the analysis of the results. Any deviation in the phase or amplitude results is assumed to be apparent as a consequence of the specific diffusion path. The diffusion through the structure is influenced by the thermal conductivity, which will be modified at damage sites such as delaminated areas. Hence the heat diffusion through the damage will be modified and data from this region will have a different phase to that from undamaged material. Therefore, the damaged region will be revealed as a deviation in a phase plot. Test Specimen Design METHODOLOGY The test specimens were manufactured using SP Systems SE84 preimpregnated UD E glass epoxy material, with various layup configurations, details of which are given later in this paper. Each test specimen was 295mm long, 100mm wide, and 1.5mm thick, and the material properties for the individual GFRP layers is given in Table 1.
4 Table 1. UD EGlass/epoxy material properties Longitudinal Young s modulus, E GPa (Measured) Transverse Young s modulus, E GPa (Measured) Shear modulus, G 12 3 GPa [10] Major Poisson s ratio, (Measured) Minor Poisson s ratio, (Measured) Coefficient of thermal expansion, C [18] Coefficient of thermal expansion, C [18] Fatigue Rig The fatigue rig was based on a design reported [12] in which a rig was developed to propagate delamination damage for acoustic fatigue studies of CFRP. The purpose of the rig was to generate interlaminar shear between neighbouring plies within the laminate. A servo hydraulic test machine was used to apply the displacement therefore the fatigue rig was designed to be mounted directly to the test machine as shown in Figure 1. The displacement of the free end of the test specimen is achieved though a roller which does not subject the laminate to a point load but generates a pure bending moment. The plan elevation in Figure 1 illustrates the clamped boundary condition designed in a half sine profile as suggested in [12]. The purpose of this clamp design is to generate higher levels of interlaminar shear in the central region of the laminate and helps initiates delamination damage away from the freeedges. Further, this avoids peeling at the freeedges of the specimen and the arrangement ensures fatigue damage initiates along the centreline. Figure 1. Fatigue rig insitu on servohydraulic test machine. Fatigue Test Routine and Experimental Procedure Figure 2a shows a laminate in the undamaged condition. For reference Figure 2b shows a UD specimen with PTFE inserts as used in [13]. As the specimens are made of GFRP, it is possible to see the PTFE and also allows any damage to be visually observed in the specimen during fatigue. The first laminate to be fatigue loaded was manufactured with a stacking sequence of [0, 45, 45] s and was subjected to cycles of fully reversed bending
5 with a displacement amplitude of 30 mm at 1 Hz. Visual inspection of the specimen revealed delamination had propagated, the extent of the damage can be seen in Figure 2c and 2d. The visual images were obtained using a digital camera and illuminating the rear of the specimen. The delamination damage achieved can be appreciated when compared to the as manufactured laminate and the laminate with pseudo delamination inserts. To reduce the number of fatigue cycles in which delamination may be initiated and propagated in laminates it was decided to manufacture specimens with stacking sequences that generated a greater shear coupling ply mismatch. This was because it has been reported that the shear stress generated in angleply laminates can have a strong influence on delamination [14]. The peak mismatch in the shear coupling coefficient occurs when the plies are orientated at about ± 20 [15]. As expected there is no mismatch in the shear coupling coefficient for cross ply laminates as the coefficient tends to zero when the plies are orientated at 0 and 90. Therefore a laminate was manufactured with a stacking sequence of [0, 25, 25] s and was subjected to cycles at 25mm displacement amplitude. The damaged laminate is shown Figure 2e and 2f and show that a significant delamination can be achieved over a much reduced fatigue period than that of the initial [0, 45, 45] s specimen. A further factor to consider is in Figure 2c, 2d, 2e and 2f surface cracking has occurred that is a result of the clamp corners causing damage to the surface plies. The clamp corners were rounded to prevent the surface damage. a) [0, 45, 45] s b) [0] 13 c) [0, 45, 45] s d) [0, 45, 45] s e) [0, 25, 25] s f) [0, 25, 25] s g) [0, 25,25, 0] s h) [0, 25,25, 0] s Figure 2. Delaminated GFRP specimens. The last laminate maintained the ± 25 angle plies within the laminate but they were separated by two 0 plies in the centre of the laminate which moved the angled plies away from the neutral axis of the laminate, resulting in a [0, 25, 25, 0] s laminate. The laminate was cycled for cycles again with 25 mm displacement amplitude. Figure 2g and 2h illustrate the delamination that was achieved. Inspection of Figure 2g and 2h (from the front and rear surface respectively) show that the delamination occurs
6 at two spatial locations through the laminate thickness; 1) between the first ± 25 laminae and 2) repeated between the second ± 25 laminae, i.e. between the 2 nd and 3 rd lamina and the 7 th and 8 th lamina from the surface ply. RESULTS AND DISCUSSION Pulsed Phase Thermography To establish the extent of the damage PPT was performed on the specimen at the end of the fatigue test routine, in reality this would determine the area that the TSA would be directed. The specimen was clamped in a vertical orientation and subjected to a metered thermal pulse using a Cullman camera flash unit positioned in contact with the rear surface of the specimen. A Cedip Silver 450M IR system was positioned 0.5 m from the front surface of the specimen and collected thermal data during the temperature decay from the surface. The basis of the setup followed recommendations of Marinetti et al. [16]. The temporal information from the sequence of 500 thermal frames recorded was analysed for the frequency content of the constituent wave forms using a Fourier transform algorithm provided in the Cedip Altair software. The frequency range over which the analysis was carried out was between 0.1 and 1 Hz. The resolution of the results was determined by the frequency increment which was set at 0.09 Hz and thus provided 11 groups. a) [0, 45, 45] s (No damage) b) [0] 13 (PTFE inserts) c) [0, 45, 45] s (Front) d) [0, 45, 45] s (Rear) e) [0, 20, 20] s (Front) f) [0,20,20] s (Rear) g) [0, 25,25, 0] s (Front) h) [0, 25,25, 0] s (Rear) Figure 3. PPT results from delaminated specimens. The defect visible in Figure 3 is provided as a function of the phase difference of a 0.5 Hz frequency wave set. The defect is visible as a result of the modification of the diffusion path, due to the damage altering the thermal conductivity, from the energy source to the surface. (The delamination is essentially an air pocket and modifies the
7 diffusion characteristics so that the damage could be visualised using the PPT technique). The phase reference is taken across the field of view with respect to the defect area. It can be seen that the defects revealed using PPT correlate well with the visual inspections in Figure 2. In all cases where delamination is present it can be seen that the PPT routine is capable of discerning the spatial extent of the subsurface damage. TSA damage analysis The thermoelastic damage analysis was conducted by obtaining thermoelastic data from the damaged laminate in the fatigue rig (Figure 1) and using the actuator displacement to cyclically load the laminate. A Deltatherm system was used to collect this data, which introduces a challenge as the laminate cannot be positioned directly in the field of view. The DeltaTherm system cannot be positioned above the fatigue rig as it must be maintained in a horizontal position due to the open storage of liquid nitrogen that is used to cool the IR detector. In [17] it was reported that a mirror could be used to collect thermoelastic data where a component was loaded horizontally; although a small reduction in the signal of 7.2 % was reported. As the attenuation is constant throughout the testing it could be incorporated in a calibration routine if necessary. The setup for the fatigue rig is shown in Figure 4. Figure 4. TSA test setup. The first laminate tested was the [0, 25,25, 0] s specimen which was cyclically displaced at 1.3 mm at 10 Hz frequency and thermoelastic data collected. The expected stress distribution due to the clamping arrangement and the bending moment applied was clearly evident in the uncalibrated thermoelastic data however it was not possible to obtain thermoelastic results that indicated any deviation in the surface stress at the known location of the subsurface damage. Thermoelastic data was also collected from the [0, 20, 20] s and [0, 45, 45] s laminates (which had been delaminated) which were also loaded at the same amplitude and frequency; the thermoelastic data depicted the gross surface cracking but provided no further indication of the subsurface damage. There are a number of reasons why the thermoelastic data did not display any variation in the signal around the delaminated area. Firstly, the delamination damage is located near the central axis of the laminate which under bending is a neutral axis and as such the damage may not effect the strain distribution within the laminate. Secondly, at 10 Hz the applied displacement amplitude was restricted to 1.3mm which may not cause
8 sufficient strain within the laminate for the damage to modify the strain distribution at the surface. It may be possible to overcome both problems by manufacturing a thicker laminate thereby allowing the angle plies to be moved further from the central axis and this would also result in a larger stress within the laminate for the achievable displacement amplitude at the required frequency. In response to the questions raised [13] during the attempt to observe pseudo delamination damage using TSA it was decided that a specimen could be fatigued in the rig and subject to TSA in uniaxial tensiontension loading. As the existence of delamination damage could be verified it would be possible to assess the response of TSA to delamination damage alone from a specimen subjected to a tensile load. To enable the specimen to be loaded between the grips of the servohydraulic test machine a narrower specimen of 45 mm width was manufactured. The specimen was subject to fatigue and TSA loading as detailed in Table 2. Table 2. Cyclic loading TSA Fatigue Specimen Displacement Frequency Displacement Frequency Cycles i) mm 10 Hz 20 mm 1 Hz 6000 Number of steps 5 For consistency however the specimen was cyclically loaded using a constant displacement and this would allow for any unanticipated reduction in stiffness. Initial thermoelastic data was obtained before the specimen was fatigued and is shown in Figure 5a. Within the noise level expected the thermoelastic data recorded is uniform across the surface. The specimen was fatigued as detailed in Table 2 over 5 steps of approximately 6000 cycles or at a stage when it was evident that damage had visibly propagated. The data in Figure 5b, 5c, 5d and 5e show influence of the progression of the damage on the thermoelastic signal and compares to the damaged area seen in the visual image in Figure 5f which shows the damage evident at the end of the test. L T a) b) Step 1 c) Step 2 d) Step 3 e) Step 4 f) Visual Figure 5. Thermoela stic signal from specimen through fatigue history. The strain data for the delaminated specimen was analysed using a damage analysis macro [15], which was written in MATLAB to provide a percentage change in the strain sum between undamaged and damaged specimen data. Two data sets are
9 compared; one from the step 1 (Figure 5b) and the other from the undamaged state (Figure 5a). The results are shown in Figure 6; the fullfield contour plot shows the regions that are affected by the subsurface delamination and in Figure 6b a line plot (as defined in Figure 5a) plots the data interrogated along the line. There are two regions of interest, from pixel 82 to 104, where the signal has increased/decreased significantly. Through the area corresponding to the delaminated region the signal is reduced by a factor of 0.8. At the delamination front there is a concentrated region of high signal 1.17 times greater than that recorded form the undamaged specimen. A further area of signal change has occurred due to the fatigue away from the delaminated area, this is located between pixels 19 to 27. This area corresponds to the section of the strip located between the rollers of the fatigue rig where damage has also accumulated. The comparison of the thermoelastic data collected from the undamaged and damaged structure demonstrates the capability of TSA to provide information on strain redistribution caused by subsurface damage. a) b) Figure 6. Thermoelastic damage analysis ratio. CONCLUSIONS A methodology has been presented to permit the integrity assessment of composite structure subject damage using two IR techniques (PPT and TSA) to provide a noncontact, nondestructive and fullfield damage assessment. This has been demonstrated on a GFRP specimen with delamination damage. A visualisation procedure highlighted the areas containing gross damage and has the potential to isolate regions were repair is necessary. ACKNOWLEDGEMENTS The authors gratefully acknowledge the Engineering and Physical Sciences Research Council for the loan of some of the IR equipment. References 1. DulieuBarton, J.M., and Stanley, P., Development and applications of thermoelastic stress analysis, J. Strain Analysis, 1998, 33,
10 2. DulieuBarton J.M., Emery T.R., Quinn S., Cunningham P.R., A temperature correction methodology for quantitative thermoelastic stress analysis and damage assessment, Meas. Sci. Tech., 2006, 17, S. Marinetti, Y.A. Plotnikov, W.P. Winfree and A. Braggiotti, Pulse phase thermography for defect detection and visualization, Nondestructive Evaluation of Aging Aircraft, Airports, and Aerospace Hardware III, SPIE Pitarresi, G. and Patterson, E. A., A review of the general theory of thermoelastic stress analysis. The Journal of Strain Analysis for Engineering Design, 2003, 38 (5), Stanley, P. and Chan, W. K., Quantitative stress analysis by means of the thermoelastic effect. The Journal of Strain Analysis for Engineering Design, 1985, 20 (3), DulieuSmith, J. M., Alternative calibration techniques for quantitative thermoelastic stress analysis. Strain, 1995, 31 (1), DulieuBarton, J. M. and Stanley, P., Development and applications of thermoelastic stress analysis. The Journal of Strain Analysis for Engineering Design, 1998, 33 (2), Stanley, P. and Chan, W. K., The application of thermoelastic stress analysis to composite materials. Journal of Strain Analysis, 1988, 23 (3), DulieuSmith, J. M., Quinn, S., Shenoi, R. A., Read, P. J. C. L., and Moy, S. S. J., Thermoelastic stress analysis of a GRP tee joint. Applied Composite Materials, 1997, 4 (5), Daniel, I. M. and Ishai, O., Engineering Mechanics of Composite Materials. 1994: Oxford University Press. 11. Maldague, X. and Marinetti, S., Pulse phase infrared thermography. Journal Applied Physics, 1996, 79 (5), Drew, R. C. and White, R. G. An investigation into damage propagation and its effect upon dynamic properties of CFRP composite materials. In Proceedings of the Fourth International Conference on Composite Structures Paisley College of Technology. 13. Cunningham, P. R., DulieuBarton, J. M., Dutton, A. G., and Shenoi, R. A., The effect of ply layup on the thermoelastic repsonse of laminated composites. Key Engineering Materials, 2002, , Herakovich, C. T., On the relationship between engineering properties and delamination of composite materials. Journal of Composite Materials, 1981, 15 (3), Emery, T.R., Identification of damage in composite materials using themoelastic stress analysis. PhD Thesis, University of Southampton, May Marinetti, S., Plotnikov, Y. A., Winfree, W. P., and Braggiotti, A., Pulse phase thermography for defect detection and visualization. Nondestructive Evaluation of Aging Aircraft, Airports, and Aerospace Hardware III, ed. Mal, A.K. Vol : Proceedings of SPIE. 17. DulieuBarton, J. M., Earl, J. S., and Shenoi, R. A., Determination of the stress distribution in foamcored sandwich construction composite tee joints. The Journal of Strain Analysis for Engineering Design, 2001, 36 (6), Harwood, N. and Cummings, W.N., Thermoelastic stress analysis. 1991, New York: Adam Hilger.
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationAnalysis of Thermal Stress in Fatigue Fracture Specimen using Lockin Thermography
Analysis of Thermal Stress in Fatigue Fracture Specimen using Lockin Thermography WonTae Kim*, ManYong Choi**, JungHak Park** * Major of Biomechanical Engineering, Kongju National University, Chungnam,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationLAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES. Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp.
LAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp. 12611266 INTRODUCTION Michael D. Seale and Barry T. Smith Departments
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationby M. Susa *, H. Benitez**, C. IbarraCastanedo *, H. Loaiza**, A. Bendada, X. Maldague*
Phase contrast using Differentiated Absolute Contrast Method by M. Susa *, H. Benitez**, C. IbarraCastanedo *, H. Loaiza**, A. Bendada, X. Maldague* * Université Laval, Québec (QC), Canada ** Universidad
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationCombined Acoustic Emission and Thermographic Testing of Fibre Composites
19 th World Conference on NonDestructive Testing 2016 Combined Acoustic Emission and Thermographic Testing of Fibre Composites Matthias GOLDAMMER 1, Markus G. R. SAUSE 2, Detlef RIEGER 1 1 Siemens AG
More informationAPPLICATION OF THERMOGRAPHY TO ANALYSIS OF THERMAL STRESS IN THE NDT FOR COMPACT TENSILE SPECIMEN
12 th APCNDT 2006 AsiaPacific Conference on NDT, 5 th 10 th Nov 2006, Auckland, New Zealand APPLICATION OF THERMOGRAPHY TO ANALYSIS OF THERMAL STRESS IN THE NDT FOR COMPACT TENSILE SPECIMEN ManYong
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationNumerical Vibration Analysis of Impacted CFRP Specimens Using COMSOL Multiphysics
Numerical Vibration Analysis of Impacted CFRP Specimens Using COMSOL Multiphysics Philipp Jatzlau 1, Florian Seybold 1 1 Technical University of Munich, Center for Building Materials, Chair of Nondestructive
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationSHOCK FOCUSING IN WATER IN A CONVERGENT CARBON FIBER COMPOSITE STRUCTURE
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS SHOCK FOCUSING IN WATER IN A CONVERGENT CARBON FIBER COMPOSITE STRUCTURE C. Wang 1, V. Eliasson 2 * 1 Department of Physics, University of Southern
More informationNew data analysis to evaluate defects in composite materials using microwaves thermography
11 th International Conference on Quantitative InfraRed Thermography New data analysis to evaluate defects in composite materials using microwaves thermography by U. Galietti*, D. Palumbo*, G. Calia* and
More informationUltrasonic Monitoring and Evaluation of Very High Cycle Fatigue of Carbon Fiber Reinforced Plastics
More 7th International Workshop NDT in Progress Fraunhofer Institute for Nondestructive Testing Dresden branch IZFPD, Germany November 78, 2013 Ultrasonic Monitoring and Evaluation of Very High Cycle
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationUniversity of Southampton Research Repository eprints Soton
University of Southampton Research Repository eprints Soton Copyright and Moral Rights for this thesis are retained by the author and/or other copyright owners. A copy can be downloaded for personal noncommercial
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationNONDESTRUCTIVE EVALUATION OF COMPOSITES MATERIALS BY PULSEDPHASE THERMOGRAPHY: DEPTH INVERSION
NONDESTRUCTIVE EVALUATION OF COMPOSITES MATERIALS BY PULSEDPHASE THERMOGRAPHY: DEPTH INVERSION Fernando López Rodríguez, flopez@cwpanama.net Vicente de Paulo Nicolau, vicente@emc.ufsc.br Hugo Oshiro,
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationApplication of thermal methods for characterization of steel welded joints
10 th International Conference on Quantitative InfraRed Thermography July 2730, 2010, Québec (Canada) Application of thermal methods for characterization of steel welded joints by U. Galietti*, D. Palumbo*
More informationDevelopment of a NDT method using thermography for composite material inspection on aircraft using military thermal imager
Development of a NDT method using thermography for composite material inspection on aircraft using military thermal imager By : P. Servais 1 and N. Gerlach 2 1 Competence Center Flying Material, Non Destructive
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationInfrared vision applications for the nondestructive testing of materials. Outline. Clemente Ibarra Castanedo. 1. Active infrared thermography
Chaire de recherche du Canada Titulaire : Xavier Maldague Infrared vision applications for the nondestructive testing of materials Clemente.Ibarra Castanedo@gel.ulaval.ca http://mivim.gel.ulaval.ca Clemente
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationLockin thermography to monitor propagation of delamination in CFRP composites during compression tests
11 th International Conference on Quantitative InfraRed Thermography Lockin thermography to monitor propagation of delamination in CFRP composites during compression tests by C. Toscano*, A. Riccio**,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationDefect Detection Capability of Pulsed Transient Thermography
Defect Detection Capability of Pulsed Transient Thermography by S. Quek, and D.P. Almond UK Research Centre in NDE, Department of Engineering and Applied Science, University of Bath, Bath, BA 7AY. email:
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationThe Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/ Laminate in Tension, Compression and Bending
The Effects of Holesize and Environment on the Mechanical Behaviour of a Quasiisotropic AS4/3506 Laminate in Tension, Compression and Bending Paul J. Callus Air Vehicles Division Defence Science and
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationConstitutive models: Incremental (Hypoelastic) Stress Strain relations. and
Constitutive models: Incremental (Hypoelastic) Stress Strain relations Example 5: an incremental relation based on hyperelasticity strain energy density function and 14.11.2007 1 Constitutive models:
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationNondestructive Evaluation of Pavements Ð Ultrasonic Tomography
Nondestructive Evaluation of Pavements Ð Ultrasonic Tomography Kyle Hoegh, Graduate Student Dr. Lev Khazanovich, Associate Professor Civil Engineering Department University of Minnesota Ð Twin Cities Outline!
More informationLASER SPOT THERMOGRAPHY FOR CRACK DETECTION IN ALUMINUM STRUCTURES
7 th International Symposium on NDT in Aerospace We.5.A.5 LASER SPOT THERMOGRAPHY FOR CRACK DETECTION IN ALUMINUM STRUCTURES Jakub ROEMER 1, Tadeusz UHL 1, Łukasz PIECZONKA 1 1 AGH University of Science
More informationMonitoring Fatigue Damage in CFRP Using Ultrasonic Birefringence
19 th World Conference on NonDestructive Testing 2016 Monitoring Fatigue Damage in CFRP Using Ultrasonic Birefringence Peter FEY 1, Marc KREUTZBRUCK 1 1 Universität Stuttgart, Stuttgart, Germany Contact
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationDIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE
DIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE Ab Ghani A. F Sustainable Maintenance Engineering Research Group, Universiti Teknikal Malaysia Melaka,
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationNumerical modelling of induced tensile stresses in rock in response to impact loading
Numerical modelling of induced tensile stresses in rock in response to impact loading M.T. Mnisi, D.P. Roberts and J.S. Kuijpers Council for Scientific and Industrial Research (CSIR): Natural Resources
More informationQuantitative Defect Reconstruction in Active Thermography for FiberReinforced Composites
19 th World Conference on NonDestructive Testing 2016 Quantitative Defect Reconstruction in Active Thermography for FiberReinforced Composites Sebastian GÖTSCHEL 1, Christiane MAIERHOFER 2, Jan P. MÜLLER
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationDETERMINATION OF CFRP S MECHANICAL PROPERTIES USING ULTRASOUND METHODS
DETERMINATION OF CFRP S MECHANICAL PROPERTIES USING ULTRASOUND METHODS Raimond GRIMBERG 1, Adriana SAVIN 1, Rozina STEIGMANN 1, Alina BRUMA 1, Paul Doru BARSANESCU 2, Daniel Petrica SALAVASTRU 2 1 Nondestructive
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationEffect of objecttocamera distance on temperature and spatial resolution of a Thermal imaging system FLIR SC 5000
Effect of objecttocamera distance on temperature and spatial resolution of a Thermal imaging system FLIR SC 5000 B. B. Lahiri, S. Bagavathiappan, John Philip, B.P.C. Rao & T. Jayakumar NonDestructive
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationFull Scale Structural Durability Test Spectrum Reduction by Truncation Coupon Testing
Full Scale Structural Durability Test Spectrum Reduction by Truncation Coupon Testing Ogewu C. Agbese F16/F22 IFG Service Life Analysis Lockheed Martin Aeronautics Fort Worth, TX, USA ogewu.c.agbese@lmco.com
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationQuantitative Defect Reconstruction in Active Thermography for FiberReinforced Composites
Zuse Institute Berlin Takustraße 7 D14195 BerlinDahlem Germany SEBASTIAN GÖTSCHEL, CHRISTIANE MAIERHOFER, JAN P. MÜLLER, NICK ROTHBART, MARTIN WEISER Quantitative Defect Reconstruction in Active Thermography
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationNONDESTRUCTIVE EVALUATION OF CONCRETE STRUCTURES BY NONSTATIONARY THERMAL WAVE IMAGING. Ropar, Nangal Road, Rupnagar, Punjab , India
Progress In Electromagnetics Research Letters, Vol. 32, 39 48, 2012 NONDESTRUCTIVE EVALUATION OF CONCRETE STRUCTURES BY NONSTATIONARY THERMAL WAVE IMAGING R. Mulaveesala 1, *, S. S. B. Panda 2, R. N.
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationThermal Vibration of Magnetostrictive Material in Laminated Plates by the GDQ Method
The Open echanics Journal, 007, 1, 937 9 Thermal Vibration of agnetostrictive aterial in Laminated Plates by the GDQ ethod C.C. Hong * Department of echanical Engineering, Hsiuping Institute of Technology,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationTHERMOELASTIC STRESS ANALYSIS TECHNIQUES FOR MIXED MODE FRACTURE AND STOCHASTIC FATIGUE OF COMPOSITE MATERIALS
THERMOELASTIC STRESS ANALYSIS TECHNIQUES FOR MIXED MODE FRACTURE AND STOCHASTIC FATIGUE OF COMPOSITE MATERIALS A Dissertation Presented to The Academic Faculty by BoSiou Wei In Partial Fulfillment of
More informationActive Thermography for Quantitative NDT of CFRP Components
2nd International Symposium on NDT in Aerospace 2010  Mo.3.A.2 Active Thermography for Quantitative NDT of CFRP Components Christian SPIESSBERGER, Alexander DILLENZ, Thomas ZWESCHPER edevis GmbH, Handwerkstr.
More information